Extraordinary optical transmission induced by electric resonance ring and its dynamic manipulation at far-infrared regime

We present a design for a sub-wavelength hole array (SHA) decorated with an electric resonance ring (ERR) to realize angle-insensitive extraordinary optical transmission (EOT) at 9.7 μm. A net electric resonance in the whole MM plane, induced by the counter-circulating LC loops in each MM unit-cell, is proposed to have the primary responsibility for the EOT. By tuning the carrier density of an added doped-semiconductor that participates in the in-plane LC resonance, dynamic EOT manipulation and an electric-control turn-on/off function is obtained in our MM. ©2011 Optical Society of America OCIS codes: (050.6624) Subwavelength structures; (160.3918) Metamaterials; (260.5740) Resonance. References and links 1. A. Sihvola, “Metamaterials in electromagnetics,” Metamaterials (Amst.) 1(1), 2–11 (2007). 2. E. Shamonina and L. Solymar, “Metamaterials: how the subject started,” Metamaterials (Amst.) 1(1), 12–18 (2007). 3. J. B. Pendry, A. J. Holden, D. J. Robbins, and W. J. Stewart, “Magnetism from conductors and enhanced nonlinear phenomena,” IEEE Trans. Microw. Theory Tech. 47(11), 2075–2084 (1999). 4. D. R. Smith and N. Kroll, “Negative refractive index in left-handed materials,” Phys. Rev. Lett. 85(14), 2933– 2936 (2000). 5. R. A. Shelby, D. R. Smith, and S. Schultz, “Experimental verification of a negative index of refraction,” Science 292(5514), 77–79 (2001). 6. S. Lim, C. Caloz, and T. Itoh, “Metamaterial-based electronically controlled transmission-line structure as a novel leaky-wave antenna with tunable radiation angle and beamwidth,” IEEE Trans. Microw. Theory Tech. 52(12), 2678–2690 (2004). 7. W. J. Padilla, A. J. Taylor, C. Highstrete, M. Lee, and R. D. Averitt, “Dynamical electric and magnetic metamaterial response at terahertz frequencies,” Phys. Rev. Lett. 96(10), 107401 (2006). 8. H.-T. Chen, W. J. Padilla, J. M. O. Zide, A. C. Gossard, A. J. Taylor, and R. D. Averitt, “Active terahertz metamaterial devices,” Nature 444(7119), 597–600 (2006). 9. T. W. Ebbesen, H. J. Lezec, H. F. Ghaemi, T. Thio, and P. A. Wolff, “Extraordinary optical transmission through sub-wavelength hole arrays,” Nature 391(6668), 667–669 (1998). 10. H. A. Bethe, “Theory of diffraction by small holes,” Phys. Rev. 66(7-8), 163–182 (1944). 11. W. L. Barnes, A. Dereux, and T. W. Ebbesen, “Surface plasmon subwavelength optics,” Nature 424(6950), 824– 830 (2003). 12. H. J. Lezec and T. Thio, “Diffracted evanescent wave model for enhanced and suppressed optical transmission through subwavelength hole arrays,” Opt. Express 12(16), 3629–3651 (2004). 13. K. Aydin, A. O. Cakmak, L. Sahin, Z. Li, F. Bilotti, L. Vegni, and E. Ozbay, “Split-ring-resonator-coupled enhanced transmission through a single subwavelength aperture,” Phys. Rev. Lett. 102(1), 013904 (2009). 14. X.Yin, C.Huang, Q.-J. Wang, and Y.-y. Zhu, “Transmission resonance in a composite plasmonic structure,” Phys. Rev. B 79(15), 153404 (2009). 15. H. Liu, T. Li, Q. J. Wang, Z. H. Zhu, S. M. Wang, J. Q. Li, S. N. Zhu, Y. Y. Zhu, and X. Zhang, “Extraordinary optical transmission induced by excitation of a magnetic plasmon propagation mode in a diatomic chain of slithole resonators,” Phys. Rev. B 79(2), 024304 (2009). 16. W. J. Padilla, M. T. Aronsson, C. Highstrete, M. Lee, A. J. Taylor, and R. D. Averitt, “Electrically resonant terahertz metamaterials: theoretical and experimental investigations,” Phys. Rev. B 75(4), 041102(R) (2007). 17. J. M. Manceau, N. H. Shen, M. Kafesaki, C. M. Soukoulis, and S. Tzortzakis, “Dynamic response of metamaterials in the terahertz regime: blueshift tunability and broadband phase modulation,” Appl. Phys. Lett. 96(2), 021111 (2010). 18. A. B. Sproul and M. A. Green, “Improved value for the silicon intrinsic carrier concentration from 275 to 375 K,” J. Appl. Phys. 70(2), 846–854 (1991). #149171 $15.00 USD Received 13 Jun 2011; revised 2 Aug 2011; accepted 16 Aug 2011; published 31 Aug 2011 (C) 2011 OSA 12 September 2011 / Vol. 19, No. 19 / OPTICS EXPRESS 18109 19. E. D. Palik and D. F. Edwards, Handbook of Optical Constants of Solids (1985). 20. W. Zhang, A. K. Azad, J. Han, J. Xu, J. Chen, and X.-C. Zhang, “Direct observation of a transition of a surface plasmon resonance from a photonic crystal effect,” Phys. Rev. Lett. 98(18), 183901 (2007). 21. A. V. Krasavin, K. F. MacDonald, N. I. Zheludev, and A. V. Zayats, “High-contrast modulation of light with light by control of surface plasmon polariton wave coupling,” Appl. Phys. Lett. 85(16), 3369–3371 (2004). 22. C. Janke, J. G. Rivas, P. H. Bolivar, and H. Kurz, “All-optical switching of the transmission of electromagnetic radiation through subwavelength apertures,” Opt. Lett. 30(18), 2357–2359 (2005). 23. J. Dintinger, I. Robel, P. V. Kamat, C. Genet, and T. W. Ebbesen, “Terahertz all-optical molecule-plasmon modulation,” Adv. Mater. (Deerfield Beach Fla.) 18(13), 1645–1648 (2006). 24. T. J. Kim, T. Thio, T. W. Ebbesen, D. E. Grupp, and H. J. Lezec, “Control of optical transmission through metals perforated with subwavelength hole arrays,” Opt. Lett. 24(4), 256–258 (1999). 25. T. Nikolajsen, K. Leosson, and S. I. Bozhevolnyi, “Surface plasmon polariton based modulators and switches operating at telecom wavelengths,” Appl. Phys. Lett. 85(24), 5833–5835 (2004). 26. S. Park and S. H. Song, “Polymeric variable optical attenuator based on long range surface plasmon polaritons,” Electron. Lett. 42(7), 402–404 (2006). 27. H.-T. Chen, H. Lu, A. K. Azad, R. D. Averitt, A. C. Gossard, S. A. Trugman, J. F. O’Hara, and A. J. Taylor, “Electronic control of extraordinary terahertz transmission through subwavelength metal hole arrays,” Opt. Express 16(11), 7641–7648 (2008).


Introduction
Meta-materials (MMs) have generated great interest [1,2] due to their ability to exhibit an artificial response not readily available in naturally occurring materials, such as artificial magnetism [3], negative refractive index [4,5], and so on.Recently, a hot field in MMs studies, which is obtaining extensive attention, is to create an active or dynamical response at many technical relevant frequencies [6].Dynamic modulations in MMs at microwave and THz regime have been realized experimentally.In 2004, Lim et al. introduced the concept of dynamic control into a composite transmission-line structure to realize a leaky-wave antenna with tunable radiation angle and beamwidth at microwave frequencies [6].Subsequently, this concept was extended to higher frequencies.For instance, Padilla et al. utilized split-ring resonator (SRR) on high resistivity GaAs substrate to realize dynamical electric and magnetic response at terahertz (THz) frequencies [7].Chen et al. developed an active THz device based on MM element [8].In their design, SRR array and n-doped GaAs substrate are combined together to effectively form a Schottky diode, which enables about an order of magnitude improvement modulation of THz transmission over existing devices.
On the other hand, optical transmission through sub-wavelength aperture has been studied continuously for centuries.Standard diffraction theory says that an aperture, whose dimensions are much smaller than the wavelength of light, would diffract light in all directions uniformly and only permits very poor optical transmission.The first step to overcome the limitation was accomplished by Ebbesen and his associates in 1998 [9].The observed enhanced transmission is several orders of magnitude more than that of the conventional prediction in periodic arranged sub-wavelength holes [10].It is generally accepted that Surface Plasmons Polariton (SPP) [9,11], a specific electromagnetic wave trapped on a metaldielectric interface, plays a crucial role on the enhanced transmission in the early experiments.While, in fact, this interpretation is still a topic of debate so far for that the excitation of SPP has been proved not to be the necessary condition for EOT.For instance, in 2004, Lezec1 et al. proved another EOT model in which the transmission is induced not by SPs coupling, but by the interference of diffracted evanescent waves on structured metallic and even nonmetallic films [12].In 2009, Aydin et al. presented split-ring-resonator-coupling enhancing transmission through a single sub-wavelength aperture [13].Yin et al. reported EOT phenomenon in periodic square holes inserted with 2D SRR array [14].Liu et al. recently showed that a magnetic plasmon propagation mode supported by a one-dimensional diatomic chain of slit-hole resonator can also lead to the enhanced transmission [15].
In this paper, we report that angle-insensitive EOT phenomenon can exist in a subwavelength hole array (SHA) decorated with a traditional electric resonance ring (ERR) [16].A net electric response, induced by MM unit-cell, is proved to be supported in the whole MM surface, which accounts for the enhanced transmission.Different from the mentioned magnetic coupling and ring-resonance-induced dipole emission in previous work [12][13][14][15], our mechanism provides a possible mean of endowing the angle-insensitive EOT with the characteristic of dynamic control at far-infrared regime when considering the tunable electromagnetic response in MMs [7,8,17].  .N ≈ × cm −3 at room temperature [18] and high-frequency dielectric constant about 11.7.At the same time, its dielectric property is described by Drude model as shown by Eq. (1) between 8 and 12 μm: m where 0 m is the mass of the free electron) [19].As a beginning, the electromagnetic responses of SHA and its ERR-decorated structure are simulated using a commercial microwave studio of CST 2006B with appropriate periodic boundary conditions, i.e., unit-cell boundary in x-z and y-z planes.In the z direction, two waveguide ports and respective open (with added space) boundary conditions are used for mimicking the incident wave and collecting transmission and reflectance data.Specially, the receiving port is far away from the MM surface (larger than 100 μm), in order to avoid the near-field effect and obtain stable transmission results.Figure 2 shows the corresponding amplitude spectrum of the SHA described in Fig. 1(a).It demonstrates that the pure SHA has poor optical transmission ability from 8 μm to 12 μm in our case.However, when we introduce ERR into the primary SHA according to the description in Fig. 1(a), and choose the polarization of incident wave to be y-direction (meaning that the electric field runs parallel with the split-wire in ERR), the corresponding simulated spectrum is remarkably changed as depicted by the red curve in Fig. 2. The amplitude bears evident enhancement at about 9.7 μm, which is almost four times that of the pure SHA.Comparing the two cases, we see that the introduced ERR may play an important role in the enhanced transmission.Additionally, we also observe that although the amplitude is slightly changed, the frequency of EOT peak almost has no shift with angle (TM wave), which demonstrates an angle-insensitive property.

Discussion
We figure out the role of ERR in our proposed structure through investigating the influence of the main parameters of ERR on the transmission behavior.As shown in Fig. 3(a), we get the dependence of the peak frequency on the width of the gap ( w ).It can be noticed that the transmission peak has obvious blueshift when the gap's width decreases from 0.5 μm to 0.2 μm in the case of fixed period and aperture dimensions.Figure 3(b) shows the influence of period ( P ) upon transmission spectrum, the space ( l ) of the gap also increases respectively in this case.We can see that the peak point moves to higher frequency (shorter wavelength) with increasing the period and space.In fact, both the gap's width and space influence the  surface.Due to the counter-excitation of the currents, the two magnetic responses would counteract each other in a single unit-cell.As a result, a net electric resonance is supported in the whole MM surface.Obviously, it is the mechanism of the EOT in ERR-decorated SHA, which is different from the case of EOT induced by the non-SPP mechanisms mentioned before [12][13][14][15].Also, such an EOT behavior is not the case of SPP where the EOT position can be calculated through the momentum matching condition 0 sin = ± where Λ is the specific period).Two apparent pieces of evidence are the blueshift of the peak frequency with increasing period as shown in Fig. 3(b), and the insensitivity of the peak frequency to incident angle as shown in Fig. 2.Although there is counteraction between two neighboring magnetic responses induced by LC current loop, the excited current still exists in the MM unit-cell.Thus, if the substrate is doped-semiconductor with high enough carrier density, it would participate in the LC loop and influence the electromagnetic coupling of our MM when the current passes through the split-gap.It may provide us a clue to realize dynamical EOT through changing the carrier density.Actually, researches on dynamic EOT have been done a lot due to the attractive possible application [20][21][22][23][24][25][26][27].However, these previous work focused on visible or THz regime, and were based on SPP mechanism which would, without doubt, be sensitive to incident angle.Dynamic and angle-insensitive EOT based on MM resonance has not been reported at far-infrared regime so far.To demonstrate this feature, a numerical experiment is carried out as follows.An additional dielectric layer is added between the composite structure and the Si substrate, which is a n-doped Si layer with thickness of 1 μm and high free-carrier density, for example, 18 7 10 ≈ × doped N cm −3 (the density level can be realized by using standard ion implantation doping process).Analogous with the method used in Ref. [8], the carrier density can be tuned by applying a bias-voltage between ERR-decorated SHA and a surrounding square copper strip as shown in Fig. 1(c).A space with distance of 50 μm is designed to make sure the strip will not influence the existing response.In this way, the nearby doped semiconductor will play as a tunable resistance to influence the in-plane LC resonance of ERR, further, influence the net electric resonance.We approximately calculate the resistance s R (for simplify, only the real part will be considered) in the effective region under the split-gap using the simple Eq. (2): where l and S represents the length and the cross-section's area of the effective region respectively.The resistance rate Hz is the collision frequency.The cross-section's area is approximately calculated by × eff w t where w is the width of the gap, and the height eff t approximately equals the space (l) of gap if we assume that the depletion process is isotropy in semiconductor.The curve in Fig. 4(c   We investigate the function of the tunable resistance when altering the carrier density from In this case, the carrier density is so high that the split-gap is almost electrically connected.Thus, the capacitance formed by the split-gap will be destroyed, which lead to that the inplane LC resonance is in a turn-off state.In other words, LC loop will not exist in ERR.As a result, the net electric resonance will not be supplied, and the EOT phenomenon disappears.Another case is the high transmission with a lower doped N , for instance

Fig. 1 .
Fig. 1.(a) Schematic drawing of SHA's unit-cell and (b) its ERR-decorated element.(c) These MM elements are adjoining arranged in square period (making sure all unit-cells are electrical connected), to form the ERR-decorated SHA on n-doped Si substrate.A surrounding metal ring with width of 1.μm is formed in the margin of the substrate, in order to apply a voltage bias between MM and the substrate.The inset shows the arrangement of the incident wave.Different incident directions are realized by tuning the angle (θ).

Figure 1 (
Figure 1(a) shows the unit-cell of a copper SHA with dimensions of 1 3 .P = μm and 1 3 .a = μm, which are much smaller than the concerned wavelength in the far-infrared regime (near 10 μm).The modification from Fig. 1 (a) to Fig. 1(b) shows the specific way to introduce ERR into SHA.The primary SHA is decorated by ERR through integrating the side metal portion of ERR with the unit-cell.ERR has dimensions of 0 4 .w = μm, 0 1 .d = μm and 0 1 .l = μm.Figure 1(c) shows the integrated structure combined with a semiconductor substrate material, which is a 300-μm-thick intrinsic Si layer with carrier density of 10 0 1 08 10.N ≈ × cm −3 at room temperature[18] and high-frequency dielectric constant about 11.7.At the same time, its dielectric property is described by Drude model as shown by Eq. (1) between 8 and 12 μm:

Fig. 2 .
Fig. 2. Respective transmission amplitude spectra of the pure SHA and ERR-decorated SHA with variable incident angle (TM wave).
is, the bigger width indicates the larger C , and the narrower space means smaller C .Thus, the resonance frequency f decreases or increases according to the formula 's width or space, respectively.

Fig. 3 .
Fig. 3. Dependence of the peak frequency on the width of split-gap (a) and period (b).In (b), the space of the gap increases from 0.1 to 0.3, respectively.Further, we investigate the current distribution and the equivalent model at the frequency of the EOT peak to analyze the electromagnetic coupling of our MM with incident wave.As shown in Fig.4(a), it is evident that in the plane of the composite structure, there are two counter-circulating currents respectively located in the two sub-regions in ERR, which are associated with two in-plane LC resonances as shown in Fig.4(b) (the split-gap and side metal portion in ERR provide the respective capacitance and inductance).Each in-plane LC resonance would induce a local magnetic response which is in the normal direction of the MM

Fig. 4 .
Fig. 4. (a) Current distribution at the EOT peak.(b) Equivalent circuit model of the in-plane LC resonance corresponding with (a).(c) Influence of the carrier density on the effective resistance in the split-gap region.The inset shows the Diagram of the n-doped Si substrate and the depletion region near the split-gap, where the grey scale indicates the carrier density.

#
149171 -$15.00USD Received 13 Jun 2011; revised 2 Aug 2011; accepted 16 Aug 2011; published 31 Aug 2011 (C) 2011 OSA ) shows that s R is obviously in inverse proportion to doped N , which means that we can utilize the dependence of s R on doped N to manipulate the LC loop as shown in Fig. 4(b).
Figure 5(a) depicts the influence of doped N on transmission of ERR-decorated SHA.It can be seen that the transmission amplitude of ERR-decorated SHA increases gradually with the decrease of doped N .Especially, the respective amplitude when doped N reaches 17 0.1 10 × cm -3 gets almost close to that in the case of intrinsic Si as shown in Fig. 2.

Fig. 5 .
Fig. 5. (a) Transmission amplitude spectra with increasing carrier density in the split-gap region.(b) Dependence of transmission amplitude on carrier density.

cm − 3 .
The results are depicted in Fig.5(b).Two obvious transmission levels are obtained.One case is the low transmission with high doped N